Presentation on theme: "Pertemuan 01 GEOSINTETIK"— Presentation transcript:
1Pertemuan 01 GEOSINTETIK Matakuliah : S0522/ Aplikasi Geosintetik Dalam Teknik SipilTahun : Juli 2005Versi : 01/01Pertemuan 01 GEOSINTETIK
2Learning OutcomesPada akhir pertemuan ini, diharapkanmahasiswa akan mampu :Mahasiswa memahami tentang geosintetik secara umum, berikut klasifikasi dan aplikasinya secara umum, sebagai tahap awal bagi desain perbaikan tanah. C2
3Outline MateriPengenalan mengenai material Geosintetik secara umum, bahan pembentuknya, polymer material dan fabrikasi, serta beberapa pengujian bahannyaKlasifikasi geosintetik menurut jenis-jenis dan material pembentuknyaAplikasi geosintetik secara umum bagi perbaikan tanah
4Geosynthetics Sebagian dari materi ini dikutip dari IGS Lecturer notes No. 3 of 20Testing of Geosynthetics byProf. Dr.-Ing. Müller-RochholzFachhochschule Münster and tBU - Institut für textile Bau-und Umwelttechnik GmbH, Greven
5Sejarah Perkembangan Geosintetik Penggunaan material alami secara konvensional, misalkan dengan menggunakan :Bahan kayuBahan jeramiBahan IjukPemadatan tanahPengertian GeosyntheticsGeo : Bumi/ tanahSynthetics : bahan sintetis / buatansehingga pengertian geosynthetics adalah :Suatu produk yang dibentuk oleh bahan polimer dan digunakan terkait dengan tanah , batuan , dan rekayasa geoteknik lainnya sebagai bagian dari proyek konstruksi.
6Sejarah Perkembangan Geosintetik Pemakaian Geosintetik terbesar dipacu pada saat pembangunan proyek Delta di BelandaOrganisasi geosintetik internasional IGS ( Internationa Geosynthetics Society , yang memiliki chapter di berbagai negara di seluruh duniahttp//………IGS Chapter Indonesia bernama Ina-IGS , memiliki sekretariat di Jurusan teknik Sipil Universitas Bina Nusantara
8Material Geosintetik Identifikasi Polimer 4oven321„5heat flowmW/mgtemperature°C61. controlled heating of oven specimen in pan 2. inert dummy in pan3. heat flow sensors4. monitor and control-PC5. result graph6.crystal melting point
10Material Geosintetik Informasi Geometris Skema2 kPa25 cm²thickness1.2.1 Thickness (ISO 9863; EN and ASTM) It is measured between plane metal plates at loads of 2, 20, 200 kPa; for product identification only the lowest load is taken.metal base
12Mass / Unit Area (mua)Mass per unit area (mua) (ISO 9864; EN 965 : 1995 ASTM) the mass per unit area is one of the most often used characteristic values, giving the price creating mass of the raw materialSpecimens are cut preferably with a circular cutter, the number depends on the specimen size; Minimum 3, each 100 cm² to a maximum of 10 specimen, and then weighed to accuracy of g and calculate the mua.100 cm²Balance .001 gmua = g/m²
13Sampling Measuring (mua) Diambil Dari IGS Lecturer notesNo. 3 of 20Testing of Geosynthetics byProf. Dr.-Ing. Müller-RochholzFachhochschule Münster and tBU - Institut für textile Bau-und Umwelttechnik GmbH, Greven
14Material Geosintetik Sifat Mekanis Short-term tensile strength and dependent deformationLong-term tensile behaviour (creep/creep rupture)Long-term compressive creep behaviour (with/without Shear stress)Resistance against impact or punchingStatic puncture test, rapid punctureResistance against abrasionFriction propertiesDirect shear, inclined plane test, pullout resistanceProtection efficiencyDamage during installationGeosynthetics or composites internal strengthGeosynthetic reinforcement segmental retaining wall unit connection testing
15Material Geosintetik Sifat Mekanis Short-term tensile strength and dependent deformation (standards see table below)
16Material Geosintetik Sifat Mekanis Capstain clamp for geogrid with laser-extensometerTesting machine with video-extensometer
18Force - Strain Behaviour of Geosynthetics HD PE - MPP/ PE - TPP - MPP/ PET - TWoven Fabrics,GeoGrids102030405060708090100strain%FmkN/m12345
19Tensile Creep and Creep Rupture EN ISO 13431 : 1996 ASTM) Tensile creep tests give information on time-dependent deformation at constant load.Creep rupture tests give time until failure at constant load.A deformation measurement is not necessary for creep rupture curves.Loads for creep testing are most often dead weights, often enlarged by lever arms.
20Creep Test Rigs – set up in a controlled environment, free from vibrations
21Multiple Creep Rupture Rigs in a Temperature Controlled Chamber
22Creep Test Results.Results are plotted for creep as linear deformation vs log time For creep rupture linear or log load vs log time. Typical curves are shownCreep RuptureCreep Curves
23Isochronus CurvesFrom creep curves at different stress grades isochronous stress strain curves may be derived or extrapolated for calculation of structure’s deformation at a given time.Isochronus curves
24Compressive Behaviour (EN ISO 13432) thickness (mm)time /h)Compressive creep random wire drainage product
25Compressive Creep Cuspated Fin Drainage Product thickness (mm)time (h)
26Creep Under Normal and Shear Stress - Cuspated Fin Drainage Product time (h)Horizontal DisplacementThickness
27Resistance To Static Puncture Static Puncture Test: The Test CBR (EN ISO : 1996) The use of soil mechanics California Bearing Ratio (CBR) apparatus for this static puncture test, has resulted in the unusual name for this test.A plunger of 50mm diameter is pushed at a speed of 50 +/- 10mm min onto and through the specimen clamped in the circular jaws. Measurement of force and displacement are taken. The test is widely used for geotextiles, it is not applicable to grids, and the test provides useful data for geomembranes.
28CBR - device in testing machine Inserting specimen in hydraulic CBR-clamps
29Typical CBR-curve force vs displacement 0.01.02.03.04.05.06.07.010.015.020.025.030.035.040.045.050.0displacement mmCBR Force kNPP - tape Fabric
30PYRAMID PUNCTURE (ASTM 5494-93) Details of Apparatus
31Dynamic Puncture Test : Cone Drop Test (ISO 13433, EN 918 : 1995) A 1kg pointed cone is dropped from a height of 1m onto a specimen, held tight in a circular clampThe diameter of a hole created is measured by means of a graduated aluminium cone scale.1. Head, release mechanism to suit laboratory requirements2. Guide rod3. Cone4. Metal screen5. Screen6. Clamping plates7. Test specimen8. Levelling screwsNote:This diagram is not to scale
33Impact Resistance Test (CEN TC 189 WI 14; ISO 13428 draft) Efficiency of protection materials can be tested by dropping a hemispherical shaped weight onto a specimen placed on a lead plate on a resilient base.The impression in the lead and the condition of the specimen are recorded. Lighter round shaped drop weights are used for other geosynthetics. The deformation of a metal sheet under the tested material gives quantitative results.
34Impact Resistance Test Drop weight, lead platen, specimen under ring
36Impact Resistance Test (performance test : BAW) A heavy drop weight (67.5 kg) is dropped from 2 m height on the geosynthetic placed on sand and fixed in a ring. The result is a “penetration yes or no” decision.2 m67.5 kgResult of drop tests - no penetrationThe Test
37Abrasion Resistance (EN ISO 13427 : 1995) Emery cloth of a specific grade is moved linearly along the specimen. After 750 cycles the abraded specimen is tested to measure the residual tensile strength or hydraulic propertiesExample of Apparatus with Sliding Block
38Specimen before testSpecimen after abrasion test
39Force vs displacement of abraded specimen (lower lines) to undamaged specimen (upper line) Force in NForce in NPP-tape fabric:Strain in %Strain in %warpweft
40Direct Shear Friction (EN ISO 12957 : 1998) Reinforcing geosynthetics develop their tensile resistance by the transfer of stresses from the soil to the fabric through friction. The friction ratio is defined as the angle of friction, the ratio of the normal stress to the shear stress. Low normal stresses may be tested by an inclined plane test and higher normal stresses by direct shear or by pull out test.Direct shear (EN ISO ) The friction partners are placed one in an upper box, the other in the lower box. The lower box is moved at a concentrate of displacement (index testing: 1 mm/min) while recording force and displacement. The results for three normal stresses (50, 100, 150 kPa) are plotted, the value of friction angle is calculated
42Inclined Plane Test (EN ISO 12957-2) The friction partners to be tested (geomembrane/geosynthetic; geomembrane/soil; geosynthetic/soil) are set up on a inclinable steel table.Movement of the upper box and inclination are measured while lifting the table by 3 degrees/min.When the upper box moves 50mm the test is stopped and the angle of the table is taken as the angle of friction for the chosen materials combination.The normal stress must be recalculated for the resulting angle at the end of the test.
44Pullout Resistance (1)A strip of the geosynthetic, just narrower than the width of the box, is pulled out of a soil filled box. A load is applied to the soil geosynthetic by pneumatic, hydraulic system or deadweight system.Force and deformation are recorded for several points of the material inside the box.
45Pullout Resistance (2)Force transfer at the point where the geosynthetic leaves the apparatus must be avoided. It is important to design a system at the front of the pullout box which avoids transferring load to the box.Results may be max force at rupture or slippage or plots of force v deformation.
46Plan view and typical gauge placement Pullout BoxPullout resistance versus percent strain of sections of pullout specimen during test
47Protection Efficiency The ability of a geotextile to protect a geomembrane is quantified by a test based on a German procedure.The deformation of a lead plate, loaded with standard M10 nuts, used as a consistently reproducible granular material. The efficiency of the geotextile to protect a geomembrane is calculated from the depth and width of the indentations.
48Protection Efficiency Arrangement of Test Apparatus
49Damage During Installation The CEN-ISO standard applies a cyclic load to a platen (100 x 200) pressing via a layer of Corundum aggregate placed on top of the geosynthetic being tested. (Corundum is a trade name for a sintered aluminium oxide.After 200 cycles between 5 kPa and 900 kPa maximum stress the specimen is exhumed and may be subject to a tensile test for the residual strength for reinforcement applications, or for filtration the hydraulic properties for filtration applications.A performance test requires the soil and fill to be used on the site and the equipment to spread and compact the material.Typical results of an index-test are shown
50Damage During Installation (ENV ISO 10722-1 : 1997) The forces applied to a geosynthetic during installation can be the most severe loading that will be applied to the material,It is therefore necessary to have a test which simulates the installation process.
51Damage During Installation Plan on apparatusFilling Corundum into upper boxCyclic loading
52Material Before (left) and After (right) Damage Test
53Geosynthetics (composites internal strength) (EN ISO 13426-1) If a failure of internal junctions may cause failure of a structure, the strength of these junctions can be tested. CEN WG 3 is developing a 3 part test.Geocells: The loading of a internal geocell-connection may be of:- a tensile shear type a peeling type a splitting type or of combinations.
55Material Geosintetik Sifat Hidraulis Water permeability characteristics normal to plane, without loadConstant headFalling headWater flow capacity in their planeCharacteristic opening size
56Hydraulic Properties: Water permeability characteristics normal to the plane, without load ( ENISO : 1999)When geosynthetics are working as filters, they are required to allow water through freely but soil grains need to be retained. Some very fine soil grains are allowed through such that a stable secondary filter is developed in the contact soil zone.The water flow may be determined at stationary (time independent) conditions i.e. constant flow at constant water head or at in stationary conditions, i.e. “falling head”.
57Constant Head TestDe-aired water passes the specimen charged with normal stresses from top to bottom (multilayer specimen of mm are used), flow vs time is measured and expressed as a kv (kn)-factor.Example of apparatus for the constant head methodIn Darcy’s equation v = kv . Iv = speed of flow (m/s)i = hydraulic gradient = head difference/specimen thickness
58Falling Head MethodDe-aired water passes the specimen charged with normal stresses from top to bottom (multilayer specimen of mm are used), flow vs time is measured and expressed as a kv (kn)-factor.Examples of apparatus for the falling head method
59Water Flow Capacity in the Plane (EN ISO 12958 : 1999) In drainage applications water needs to flow in the plane of the geosynthetic. Tests according to EN-ISO or ASTM differ in specimen size, but use the same basic principles.1 water supply 2 water collection 4 specimen 7 foam 8 load 9 loading platen 10 overflow weirs at hydraulic gradients 0,1 and 1,0water reservoirbaseTypical Example of Apparatus
60CEN - apparatus in plane flow Specimen in apparatus, net core with soft contact faces
61Typical examples of in-plane water flow capacity curves Flow is measured at constant water head and expressed either as kH (kp), unit m/s, or as flow capacity, unit l/s per m width of the product at given gradient. The flow value is dependent on the thickness of the product, as some products compress under load the flow values are time dependant.For a long-term design, flow values need to be corrected for the compressive creep of the product..Typical examples of in-plane water flow capacity curvesNormal compressive stress (kPa)
62Characteristic Opening Size (EN ISO 12956 : 1999) To determine, which grain size can passing through a geosynthetic and which is retained, a wet sieving test is used with a standard “soil”.The ‘soil’ passing the geotextile is extracted from the water and sieved again.A characteristic value O90- is calculated according to EN ISOO90 = d90 of the ‘soil’ passing the geosynthetic
64Tests according to other standards use single grade soil sand or glass-spheres to measure similar properties.090cumulative percentage passed (%)sieve opening size (µm)Cumulative curve of the granular material passed through the specimen and determination of O90
65Material Geosintetik Sifat Ketahanan/ Durability Resistance to weatheringResistance to microbiological degradation (soil burial)Resistance to liquidsResistance to hydrolysisResistance to thermal oxidation
66Durability Properties Geosynthetics may be used for temporary structures such as access roads for construction sites or may be required for medium term applications until consolidation of soils makes them redundant. Long-term applications are the main use (30 to 60 years for some in UK application or ; more than 120 years for landfills in most countries). Therefore durability is an important requirement.
67Resistance to Weathering (prEN 12224 : 1996) Products exposed uncovered to light and products placed without cover-soil for service are tested by artificial weathering.Exposure to UV-light of defined emission spectrum and rain at elevated temperature accelerates the test.
68Exposure to Natural Weathering Tensile tests after exposure and reference to fresh specimen tensile strength loss in %. Tensile tests on exposed and fresh specimens can be used to determine the loss of tensile strength, normally expressed as a percentage of strength retained after exposure.
69Resistance to Microbiological Degradation (ENV 12225 : 1996) Fungi and bacteria living in soils may attack the polymeric materials used as geosynthetics. (There are no recorded failures of geosynthetics due to micro-biological attack).To check the resistance the product to be tested they are buried in biologically active soil and after the “soil burial” test residual strength is measured. ENV gives types of bacteria and environments be used.
70Resistance to Liquids (ENV ISO 12960) The chemical tests developed to date are:the resistance to hydrolysis for Polyester based geosyntheticsand the resistance to thermal oxidation for geosynthetics made from Polyolefines.
72Resistance to Thermal Oxidation (prEN ISO 13430) To the polyolefine molecules of PE, PP oxygen may be connected creating increased brittleness of the polymers.Stabilizing additives delay this oxidation.For the test the products are exposed to high temperature in an oven.
73Resistance to Hydrolysis (pr EN 12447) Hydrolysis of Polyester is the reverse action of the evolution by polycondensation and means connecting water molecules or parts to the PET molecules, thus increasing the Carboxyl end group (CEG)-content and decreasing the average molecular weight often expressed as solution viscosity.External hydrolysis by alkaline attack occurs also at low temperatures, internal hydrolysis in neutral environments is relevant at elevated temperatures.Products are immersed in liquids for times up to 90 days and residual strength and deformation are tested.